International Journal of Science and Research (IJSR), India Online ISSN: 2319-7064
Characterization of Mn2+ ion Doped KCdBSi (K2O CdO - B2O3 – SiO2) Glasses on the Basis of Optical and Physical Properties Keerti Marita .G1, 2, Sandhya Cole1 1
Acharya Nagarjuna University, Nagarjuna nagar, Guntur, India
Godavari Institutes of Engineering and Technology, Chaitanya nagar, Rajahmundry, E G Dt, India
Abstract: K2O - CdO - B2O3 – SiO2glasses containing different concentrations of MnO2 have been prepared. The Physical properties of the glasses are studied from their density. The studies have been analysed in the light of different oxidation states of manganese ion with the aid of the data from optical absorption. The analysis shows that manganese ions exist mainly in Mn2+ state, occupy tetrahedral positions and increase the insulating strength of the glass if MnO2 is present in smaller concentrations.
Keywords: Boro silicate glass, density, optical basicity, optical absorption.
1. Introduction More recently, there has been a great deal of interest on the preparation and characterization of a wide variety of optical glasses comprising of oxides, silicates, borates, phosphates, fluorides etc., for their potential applications .Glasses based on borates and silicates have been identified as ideal optical systems because of their good glass forming ability, hardness, transparency and resistance towards moisture without any degradation on their surfaces.In order to improve the quality of glass and its optical performance from borosilicate glasses, suitable quantity (5mol %) of CdO have been added separately as the network modifier (NWF).Transition metal ions are incorporated into these borosilicate glasses in order to characterize their optical behaviours. Glasses containing transition metal ions have become the subject of interest owing to their potential applications , exhibit interesting spectroscopic properties and hence are highly suitable for solid state lasers. Electronic and magnetic properties of these glasses depend on the relative proportion of different oxidation states of transition metal ions  and their near environments in the host. In the present study, we have calculated the physical properties and optical properties of KCdBSi (K2O - CdO B2O3 – SiO2) glasses doped with a small amount of paramagnetic impurity MnO2.
2. Glass preparation and measurements The glass samples studied in the present work (Table 1) have been obtained by the classical melt quenching technique. They are prepared by mixing and grinding together appropriate amounts of K2O , CdO , B2O3, SiO2 and MnO2 in an agate mortar before transferring to a silica crucible and heating in an electric furnace in air at 1280K for half an hourThe melt is then quenched at room temperature in air by pouring it onto a polished plate. Glasses obtained are with good optical quality and high transparency. The polished glasses are used for measurements.
The physical properties are calculated by measuring density of the glasses.The density of glass samples is determined by using Archimedes’ principle with Xylene as an inert buoyant liquid. Optical absorption spectra are recorded at room temperature on JASCO V-670 Spectrophotometer with 200900 nm. Table 1: Glass compositions of Mn2+ ion in KCdBSi glass system Glass system Mno Mn1 Mn2 Mn3 Mn4
K2O CdO B2O3 SiO2 MnO2 (mol %) (mol %) (mol %) (mol %) (mol %) 20 5 60 15 19.9 5 60 15 0.1 19.8 5 60 15 0.2 19.7 5 60 15 0.3 19.6 5 60 15 0.4
3. Results and Analysis 3.1. Physical Properties From the measured values of density D, and calculated average molecular weight M, various physical parameters such as manganese ion concentration Ni and mean manganese ion separation ri for these glasses are determined using the conventional expressions and are presented in Table 1 The density of the glasses is found to increase considerably with the concentration of MnO2. The increase of structural compactness, the modification of the geometrical configuration of the glassy network, changes in the coordination of the glass forming ions are the some of the factors that are responsible for the observed increase in the density. 3.2 Optical basicity of the glass (Λth) The theoretical optical basicity (Λth) is expressed in terms of the electron density carried by oxygen. Simultaneously, an intrinsic relationship exists between the electronic
Volume 2 Issue 8, August 2013 www.ijsr.net
International Journal of Science and Research (IJSR), India Online ISSN: 2319-7064 polarizability of the oxide ions and the optical basicity of the oxide medium. An increase in the oxide ion polarizability shows stronger electron donor ability of the oxide ions and vice - versa. The theoretical values of optical basicity (Λth) of the glass can be estimated by using the formula. n
th i 1
zi 2 i
(1) where n is the total number of cations present, Zi is the oxidation number of the ith cation, ri is the ratio of number of ith cations to the number of oxides present and γi is the basicity moderating parameter where n is the total number of cations present, Zi is the oxidation number of the ith cation, ri is the ratio of number of ith cations to the number of oxides present and γi is the basicity moderating parameter of the ith cation. of the ith cation. γican be calculated from the following equation.
i 1.36 xi 0.26
Table 2: Physical parameters of Mn2+ ion in KCdBSi glass system 2.478 2.584 2.587 2.57 2.58 2.548 Density Manganese ion 1.88 3.88 5.51 7.47 9.71 concentratio(Ni) (1019ions/cm3) (±0.015) Interionic distance (ri) A0 37.6 29.58 26.27 23.74 21.76 (±0.005) 0 Polaron radius A (±0.005) - 15.15 11.92 10.58 9.56 8.77 - 0.432 0.432 0.432 0.432 0.432 Optical basicity 80.17 80.12 80.07 80.01 79.97 79.96 Avg.mol Wt.(M)
where xi is the Pauling electronegativity of the cation. The optical basicity can be used to classify the covalent/ionic character of the glasses since an increasing Λth indicates decreasing covalence. The theoretical values of optical basicity (Λth) were calculated for all the glass samples and are presented in Table 2. 3.3 Optical Absorption Studies The UV- visible absorption spectra of manganese doped KCdBSi glass samples in the wavelength region 350-900 nm is shown in Fig.1. It’s observed that, two bands are formed at 720 and 450 nm. The bands observed at 720 and 450 nm are assigned to the transitions 6A1g(S) → 4T1g (G) and 6A1g(S) → 4 T2g (G). The analysis shows that manganese ions exist mainly in Mn2+ state, occupy tetrahedral positions and increase the insulating strength of the glass if MnO2 is present in smaller concentrations. It shows a strong broad band centered at around 450 nm , [4, , and another weak band at 720nm. In general the optical spectra have been analysed in the framework of crystal field theory , . The excited quartet states 4G, 4P, 4D and 4F of Mn2+ ions in the octahedral crystal field are situated above the ground 6 S state and the trigonal crystal field splits the four levels into ten sublevels. Hence, all the transitions from the ground sextet 6S to the excited levels are spin-forbidden, the intensity of optical absorption lines of Mn2+ are weak and in addition, the Mn2+ ion had a 3d5 configuration. The broad absorption band with the maximum at around 450 nm is assigned to spin-allowed 5Eg→5T2g transition of Mn3+ (3d4, 5 D0) ions in the octahedral sites of host glass. Furthermore, this band was asymmetric, indicating that the octahedral ligand field had suffered a tetrahedral deformation by the Jahn-Teller effect. The most common manganese ions found in oxide glass are Mn2+. The most important information resulting from the analysis of optical spectra is the increase of absorption band intensity depends on the host glass basicity (Table 2). This concludes that the structural factor plays an important role in the formation of valence and coordination state of manganese ions in host glass system.
Figure 1: Optical absorption bands ofMn2+ ion doped KCBSi glass system. 3.4. Optical band gap (Eg) and Urbach energy (ΔE) The study of optical absorption and particularly the absorption edge is a useful method for the investigation of optically induced transitions and electronic band structure in both crystalline and non-crystalline materials. The principle of this technique is that a photon with energy greater than the band gap energy will be absorbed . It is calculated by extrapolating the linear region of the graph towards X-axis. The optical band gap of all the glass samples were obtained from their ultraviolet absorption edges by plotting(αhν)2, (αhν) ½, as a function of photon energy hν as shown in Figs.2,3.The values have been calculated by extrapolating the linear region of the graph towards X-axis.
Figure 2: Direct bands of Mn2+ ion doped KCdBSi glass system
Volume 2 Issue 8, August 2013 www.ijsr.net
International Journal of Science and Research (IJSR), India Online ISSN: 2319-7064 The absorption coefficients in Urbach’s tail region have been given as a function of photon energy by the equation  h 0 exp E
Where αo is a constant, ΔE is the Urbach energy interpreted as the energy gap between localized tails in the forbidden region.
Table 3: Observed band positions, optical band gap and Urbach energies for Mn2+ ions in KCdBSi glass system Band positions Glass Cut off Wave length 6A1g(S→4T1g 6A1g(S→4T2g (G) (G) Mn1 360 450 692 Mn2 362 445 685 Mn3 354 448 680 Mn4 362 439 685 Mn5 356 457 678
Optical band gap Urbach (eV) energies Direct Indirect 1.39 1.44 1.49 1.56 196
2.31 2.57 2.64 2.69 2.81
0.447 0.395 0.384 0.373 0.361
4. Conclusions 1. The physical parameter - density shows a small increase and decrease in its value by the introduction of MnO2 into the KCdBSi glasses. 2. The optical basicity remains the same for all the glasses. 3. The Optical band gap energy and the Urbach energy (ΔE) are found to be dependent upon the variation of manganese content. 4. From the results of Optical absorption spectra of Mn2+ ions in the above glasses, it is concluded that the site symmetry of the Mn2+ ion is tetragonally distorted octahedral. Figure 3: Indirect bands of Mn2+ ion doped KCdBSi glass system The Urbach energy has been calculated for all the glass samples by taking the reciprocal of the slope of the linear region in the plot drawn between lnα vs hν as shown in Fig.4.The values of the optical energy gap and Urbach energy calculated in the present work for all the glass samples are of the same order reported in the literature for borate glasses , , , and are given in Table 3.
Figure 4: Urbach plots of Mn2+ ion doped KCdBSi glass system From the table, it is observed that the decrease in optical band gap (Eg) and increase in Urbach energy (ΔE) with increase of manganese content. This is due to the shift of UV absorption band to longer wavelengths corresponds to transitions from the non-bridging oxygen which bind an excited electron less tightly than a bridging one. The KCdBSi: Mn0 sample has the least Urbach energy (0.18 eV). This suggests that defects in these glasses are at a minimum.
Shelby J E and Downie L K “ Introduction to Glass science and Technology” Phys. Chem. Glasses pp. 30, 1989.  ElbatalFatma et al. “Gamma ray interaction with lithium borate glasses containing WO3” Indian Journal of pure and applied physics. pp 471- 480, 2009.  R. P. Sreekanth Chakradhar et al. “EPR and optical investigations of manganese ions in alkali lead tetraborate glasses” Spectrochim. Acta Part A, pp.761768, 2005.  H. W. de Wijn , R.F. Van balderen , “Electron Spin Resonance of Manganese in Borate Glasses,” J. Chem. Phys, pp.1381-1387, 1967  I. E. C. Machado et al, “Optical properties of manganese in barium phosphate glasses,” J. Non-Cryst. Solids, pp. 113-117, 2004.  D.T. Sviridov, et al, “Optical spectra of transition metal ions in crystals”, Nauka, Moscow, 1976.  B. Henderson, “Crystal- field engineering of solid-state laser materials”, Cambridge Press, Cambridge, 2000.  R. P. Sreekanth Chakradhar, “Mixed alkali effect in Li2O-Na2O-B2O3 glasses containing CuO-An EPR and Optical study”, J. Non- Cryst. Solids, pp.38643871, 2006.  A. Murali, J.L. Rao, "Spectroscopic investigations on Cu(II) ions doped in alkali lead borotellurite glasses" J. Phys: Condens. Matter, pp. 7921-7935, 1999.  A. A. Kutub, M. M. EI- Samanoudy “A Study of the Optical Properties of Sodium Tetraborate Glasses Containing Ytterbium”, J. Mater. Sci., pp. 3930-3935, 1995.
Volume 2 Issue 8, August 2013 www.ijsr.net
International Journal of Science and Research (IJSR), India Online ISSN: 2319-7064 Author Profile Keerti Marita. G received M. Sc (Physics) and M. Phil degrees from Andhra University, Vizag, India, with first class in the years 1996 and 2008 respectively. She even completed her B.Ed degree. She is a being working as assistant professor in Engineering Physics in Godavari Institute of Engineering and technology. She has participated in number of seminars workshops and published nearly 20 papers. Presently she is pursuing Ph. d (Glass Science) from Nagarjuna University. Dr. Sandhya Cole is Assistant Professor in Acharya Nagarjuna University. Her areas of specialization are Glass Science, Solid State Spectroscopy, Nano Materials. She has 10 International publications (Peer Reviewed). She has attended 20 conferences/seminars/workshops. Under her guidance one- Ph. D, four-MPhil are awarded and eight more Ph. Dâ€™s and three more M. Phil are pursuing.
Volume 2 Issue 8, August 2013 www.ijsr.net